advertisement

ARTICLE IN PRESS Journal of the Mechanics and Physics of Solids 56 (2008) 3224–3241 Contents lists available at ScienceDirect Journal of the Mechanics and Physics of Solids journal homepage: www.elsevier.com/locate/jmps Mechanics of hydrogen storage in carbon nanotubes Y.L. Chen a, B. Liu a,, J. Wu a, Y. Huang b,c,, H. Jiang d, K.C. Hwang a a FML, Department of Engineering Mechanics, Tsinghua University, Beijing 100084, China Department of Civil and Environmental Engineering, Northwestern University, Evanston, IL 60208, USA c Department of Mechanical Engineering, Northwestern University, Evanston, IL 60208, USA d Department of Mechanical and Aerospace Engineering, Arizona State University, Tempe, AZ 85287, USA b a r t i c l e i n f o abstract Article history: Received 23 April 2008 Received in revised form 12 July 2008 Accepted 17 July 2008 A continuum mechanics model is established for hydrogen storage in single- and multiwall carbon nanotubes (CNTs) and the bundle of single-wall CNTs. The model accounts for the deformation of CNTs, and van der Waals interactions among hydrogen molecules and between hydrogen and carbon atoms. The analytical expressions of hydrogen storage (number of hydrogen molecules per unit volume) in CNTs are obtained, and are validated by atomistic simulations. CNTs are categorized as tiny, small, medium and large CNTs; tiny CNTs cannot achieve the goals of hydrogen storage (62 kg/m3 and 6.5 wt% of hydrogen set by the US Department of Energy) without fracture; small CNTs are strained during hydrogen storage; medium CNTs can achieve the above goals without the strain and do not self collapse; and large CNTs may self collapse upon the release of hydrogen. & 2008 Elsevier Ltd. All rights reserved. Keywords: Hydrogen storage Carbon nanotube Continuum model Analytical solution Atomistic simulations 1. Introduction Hydrogen is the cleanest vector of energy. Vehicles propelled by electric motors supplied by hydrogen fuel cells may reach zero emission, and therefore do not cause urban pollution. One challenge in this development is the storage and release of hydrogen. Carbon nanotubes (CNTs) display superior mechanical properties and have many potential applications. One of them is the hydrogen storage (Darkrim et al., 2002) because (i) carbon is a good adsorbent for gases; and (ii) CNTs are microporous carbon macromolecules with high speciﬁc surface, and have the potential to adsorb hydrogen in their nanostructures (Darkrim et al., 2002). Dillon et al. (1997) measured the hydrogen adsorption in CNTs in order to evaluate the hydrogen adsorption amount delivered during the gas desorption, and concluded that CNTs were promising for hydrogen storage. Liu et al. (1999) investigated the hydrogen adsorption in CNTs at room temperature and reached the same conclusion. Darkrim and Levesque (1998, 2000) computed hydrogen adsorption in opened CNTs for a wide range of pressure and temperature, and optimized the tube diameters and the inter-tube spacing to achieve high adsorptive property. The adsorption is expressed as a unit of quantity of gas with respect to a unit of quantity of adsorbent. Experiments have shown large scatting in the achievable hydrogen storage, ranging from 0.25 to 11 wt% (e.g., Dillon et al., 1997; Liu et al., Corresponding authors. E-mail addresses: [email protected] (B. Liu), [email protected] (Y. Huang). 0022-5096/$ - see front matter & 2008 Elsevier Ltd. All rights reserved. doi:10.1016/j.jmps.2008.07.007 ARTICLE IN PRESS Y.L. Chen et al. / J. Mech. Phys. Solids 56 (2008) 3224–3241 3225 1999; Ye et al., 1999; Rajalakshmi et al., 2000; Wu et al., 2000; Dai et al., 2002). Multi-wall CNTs doped with Li, Kt and Pd may achieve higher hydrogen storage, ranging from 1.8 to 20 wt% (e.g., Chen et al., 1999; Yang, 2000; Mu et al., 2006). Many factors may be responsible for the large scatting in experimental data, such as the defects in CNTs, and opened or closed CNTs. The goals of hydrogen storage set by the US Department of Energy are 62 kg H2/m3 and 6.5 wt% (Dillon et al., 1997). The purpose of this paper is to establish a simple mechanics model of hydrogen storage in CNTs. The model provides the analytical relation between the hydrogen storage (number of hydrogen molecules per unit volume) and the internal pressure in the CNT for single-, double- and triple-wall CNTs and bundle of single-wall CNTs. For each type (single-, double, triple-wall, and bundle), CNTs can be categorized as tiny, small, medium and large CNTs, which, upon reaching the above goals of hydrogen storage (and then release of hydrogen), will experience fracture, strain, no strain (and do not self collapse) and self collapse, respectively. The model, which is validated by atomistic simulations, also provides the analytical relation between the maximum hydrogen storage and CNT radius. The paper is structured as follows. The interatomic potentials for carbon and for van der Waals interactions are given in Section 2. The mechanics models of hydrogen storage are established in Sections 3–5 for single-wall CNTs, their bundles, and multi-wall CNTs, respectively, and are validated by atomistic simulations. The goals of hydrogen storage in CNTs are discussed in Section 6. 2. Interatomic potentials Brenner et al. (2002) established the second-generation interatomic potential for carbon as Vðr ij ; yijk ; kai; jÞ ¼ V R ðr ij Þ Bij V A ðr ij Þ, (2.1) ar P3 bn r where rij is the distance between atoms i and j, V R ðrÞ ¼ 1 þ Q =r Ae f c ðrÞ and V A ðrÞ ¼ n¼1 Bn e f c ðrÞ are the repulsive and attractive pair terms (i.e., depending only on rij), A, Q, a, Bn and bn are constants, fc is the cut-off function, and the multiP body coupling parameter Bij ¼ ½1 þ kðai;jÞ Gðcos yijk Þf c ðr ik Þ1=2 depends on the bond angle yijk between i–j and i–k via the function G. The van der Waals interactions between a carbon atom and a hydrogen molecule or between two hydrogen molecules are characterized by the Lennard–Jones 6-12 potential ! V LJ ¼ 4 s12 r 12 ij s6 r 6ij , (2.2) 6 6 where rij is the distance between atoms (and molecules), s12 =r 12 ij and s =r ij represent the repulsive and attractive terms, respectively. For hydrogen molecules, H2 H2 ¼ 3:11 103 eV and sH2 H2 ¼ 0:296 nm (Gu et al., 2001). For a carbon atom pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ and a hydrogen molecule, the Lorentz–Berthelet mixing rule (e.g., Allen and Tildesley, 1987) gives C2H2 ¼ C2C H2 2H2 ¼ 3 3 2:73 10 eV and sC2H2 ¼ 12ðsC2C þ sH2 2H2 Þ ¼ 0:319 nm, where C2C ¼ 2:39 10 eV and sC2C ¼ 0:342 nm (Gu et al., 2001; Frankland et al., 2003). 3. Hydrogen storage in single-wall CNTs 3.1. Atomistic model of hydrogen storage in single-wall CNTs Fig. 1(a) shows the atomistic model used in the prior molecular dynamics simulations of hydrogen storage in single-wall CNTs (e.g., Cheng et al., 2001, 2004; Gu et al., 2001; Dodziuk and Dolgonos, 2002). The covalent bonds between carbon atoms on the CNT are characterized by the interatomic potential in Eq. (2.1). The carbon atoms interact with the hydrogen molecules inside the CNT via the van der Waals forces obtained from Eq. (2.2) with C2H2 ¼ 2:73 103 eV and sC2H2 ¼ 0:319 nm, while hydrogen molecules also interact via the van der Waals forces with H2 2H2 ¼ 3:11 103 eV and sH2 2H2 ¼ 0:296 nm. Both carbon atoms and hydrogen molecules are discrete in the atomistic model. The atomic-scale ﬁnite element method (AFEM) (Liu et al., 2004a, 2005), which is an effective and robust atomistic simulation method based on the second-generation interatomic potential for hydrocarbons (Brenner et al., 2002), is adopted. It models each atom or molecule as a node, and accurately describes the C–C covalent bonds, and C–H2 and H2–H2 van der Waals interactions. The hydrogen molecules are randomly added inside the CNT. The system is then relaxed to minimize the total energy (in the covalent bonds and due to van der Waals interactions), which determines the positions of carbon atoms and hydrogen molecules. Fig. 2 shows the internal pressure p in the CNT versus the percentage of change of CNT radius, DR/R, for a (5,5) CNT. Here the new radius of CNT R+DR is obtained by averaging the positions of carbon atoms in the radial direction. The pressure is the ratio of total force (in the radial direction) of all carbon atoms to the current area of the CNT surface. The nonlinear pDR/R relation results from the nonlinear atomistic interactions. The peak pressure corresponds to the CNT fracture (breakage of a C–C bond). The maximum hydrogen storage at the peak pressure is 25.6 hydrogen molecules/nm3. This gives 85.0 kg H2/m3 and 3.75 wt% for the (5,5) CNT, which exceeds the goal 62 kg H2/m3 but falls short to reach the other goal 6.5 wt% of hydrogen storage [set by the US Department of Energy, see Dillon et al. (1997)]. Therefore, large CNTs (large radius) are needed for hydrogen storage. ARTICLE IN PRESS 3226 Y.L. Chen et al. / J. Mech. Phys. Solids 56 (2008) 3224–3241 Fig. 1. Schematic diagrams of hydrogen storage in single-wall carbon nanotubes: (a) atomistic model (AFEM), in which carbon atoms and hydrogen molecules are discrete; (b) continuum model, in which carbon nanotubes are represented by a continuum shell, while hydrogen molecules are represented by the internal pressure. (5,5) CNT Peak pressure 80 Pressure (GPa) 70 60 50 Continuum model Atomistic model (AFEM) 40 30 20 10 0 0.00 0.02 0.04 0.06 0.08 0.10 0.12 0.14 0.16 ΔR/R Fig. 2. The pressure inside the single-wall (5,5) carbon nanotube versus the percentage change of nanotube radius for the atomistic (AFEM) and continuum models. The peak pressure is denoted. 3.2. Continuum model of hydrogen storage in single-wall CNTs For large CNTs the atomistic model becomes less effective. The continuum model is developed in this section to establish a simple, analytical expression for hydrogen storage in single-wall CNTs. Fig. 1(b) shows the continuum model in Section 3.2.1 to represent the CNT as a continuum shell. The hydrogen molecules in the CNT are represented by the internal pressure p. A simple analytical relation is established in Section 3.2.2 to give the average spacing between hydrogen ARTICLE IN PRESS Y.L. Chen et al. / J. Mech. Phys. Solids 56 (2008) 3224–3241 3227 molecules in the CNT in terms of the internal pressure p. A similar relation is established in Section 3.2.3 to relate the average spacing between the CNT wall and nearest hydrogen molecules to the internal pressure p. As p increases, the H2–H2 spacing and C–H2 spacing decrease, but the CNT radius increases, which lead to the increasing hydrogen storage in Section 3.3.4. 3.2.1. Continuum modeling of the CNT The CNT is modeled as a nonlinear continuum thin shell (Fig. 1(b)), where the nonlinearity results from the large stretch of C–C bonds due to hydrogen storage, as characterized by the interatomic potential, Eq. (2.1). Zhang et al. (2002, 2004) and Wu et al. (2008) established a continuum theory for CNTs directly from the interatomic potential, similar to the previously developed Virtual-Internal-Bond model for cohesive fracture (Gao and Klein, 1998) but accounting for the atomic structure and multi-body atomistic interactions. This atomistic-based continuum theory is brieﬂy summarized in the following. The Cauchy–Born rule (Born and Huang, 1954) equates the strain energy at continuum level to the energy stored in atomic bonds. The atoms subjected to a homogeneous deformation move according to a single mapping F ¼ qx/qX from the initial, undeformed to the current, deformed conﬁgurations, where X and x denote positions of a material point in the initial and current conﬁgurations, respectively. A bond between a pair of atoms i and j in the initial conﬁguration is described by a vector rðij0Þ ¼ r 0 n, where r0 is the initial bond length and n is the unit vector along the initial bond direction. For a simple Bravais lattice, the deformed bond is rij ¼ F rijð0Þ , which has the length qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ð0Þ r ij ¼ r ð0Þ n ðI þ 2EÞ n, where E ¼ 12ðF T F IÞ is the Green strain tensor and I is the second-order ij ðI þ 2EÞ rij ¼ r 0 identity tensor. The single mapping F ensures the equilibrium of atoms for a simple Bravais lattice. A CNT, however, is a Bravais multi-lattice that can be decomposed into two simple Bravais sub-lattices as shown by the open and solid circles in Fig. 3. Each sub-lattice follows the single mapping F, but the two sub-lattices may have a shift f (Fig. 3) to be determined from the equilibrium of atoms. The deformed bond (between atoms from two different sublattices) then becomes rij ¼ F rijð0Þ þ f. (3.1) This gives the bond length rij and angle yijk in terms of the Green strain E as r 2ij ¼ r 20 ðdab þ 2Eab Þðna þ Za Þðnb þ Zb Þ, cos yijk ¼ (3.2) r 20 ð2Þ ðd þ 2Eal Þðnð1Þ a þ Za Þðnl þ Zl Þ, r ij r ik al (3.3) where g ¼ ð1=r 0 ÞF 1 f, and the superscripts 1 and 2 denote the two bonds in a bond angle. The strain energy density W in the continuum theory is obtained from the interatomic potential V via the Cauchy–Born rule, P 1 Vðr ij ; yijk ; kai; jÞ , (3.4) W¼ A0 2 where the summation is for three nearest-neighbor atoms, the factor one half results from the equi-partition of bond energy, and A0 is the area of CNT per atom. It is important to point out that the above equation accounts for the effect of second-nearest-neighbor atoms via the bond angle yijk. The shift vector f (or g) is determined numerically from the D A' z A C B Fig. 3. The decomposition of a hexagonal lattice to two triangular sub-lattices. A shift vector f between two sub-lattices is introduced to ensure the equilibrium of atoms. ARTICLE IN PRESS 3228 Y.L. Chen et al. / J. Mech. Phys. Solids 56 (2008) 3224–3241 equilibrium of atoms as qW qW ¼ ¼ 0. qf qg (3.5) The second Piola–Kirchhoff stress T is related to the Green strain E by Tt ¼ qW , qE (3.6) where the stress appears together with the CNT thickness t since the strain energy density W in Eq. (3.4) is the strain energy per unit area, and is also obtained numerically. The pressure in the current conﬁguration is obtained from the equilibrium as p¼ T yy t , Rð1 þ zz Þ (3.7) where the (nominal) strain ezz in the axial direction is determined numerically from Tzz ¼ 0. Fig. 2. shows the internal pressure p in the CNT versus the percentage of change of CNT radius, DR/R, for the (5,5) CNT. The continuum model gives the same curve as the atomistic model, which means that the CNT can indeed be represented by a thin shell in the continuum model. Only the peak pressure (after which the stress–strain curve displays the softening behavior) given by the continuum model is slightly higher than the atomistic model. This is because the CNT is subjected to the uniform internal pressure in the continuum model, while the atomistic model is nonuniform (due to hydrogen molecules), which may trigger earlier bond breakage. For small deformation the above continuum model becomes linear elastic isotropic, and therefore simple, analytical solution. Its constitutive model becomes (Huang et al., 2006) ! 2 1 q V ðsyy þ szz Þt ¼ pﬃﬃﬃ ðyy þ zz Þ, 3 qr 2ij 0 ðsyy szz Þt ¼ B pﬃﬃﬃ ðyy zz Þ, 8 3 (3.8) where V is the interatomic potential in Eq. (2.1), the subscript ‘‘0’’ denotes the values at the initial equilibrium state, rij ¼ r0 and yijkE1201, B is given in terms of the derivatives of the interatomic potential at the initial equilibrium state as " ! ! # 3ð1 AÞ2 qV q2 V q2 V 4 þ6 3 B¼ q cos yijk 0 q cos yijk q cos yijk q cos yijk q cos yijl r 20 0 ! ! 0 2 2 2 q V ð1 A Þ q V 12 , (3.9) þ 4ð1 þ AÞ2 qrij q cos yijk r0 qr 2ij 0 0 and 8r 20 A¼1 q2 V qr 2ij þ 12r 0 q2 V qr ij q cos yijk 0 0 . 2 2 2 2 q V q V q V 2 12 q cos y þ 4r 0 qr2 þ 18 q cos y qV cos y 9 q cos yq Vq cos y þ 12r 0 qrij qqcos y ijk 0 ij 0 ijk ijk 0 ijk ijl 0 ijk (3.10) 0 The equilibrium bond length is obtained by minimizing the potential qV=qr ij r ¼r ; y 120 ¼ 0 as r0 ¼ 0.142 nm for the 0 ij ijk second-generation interatomic potential (Brenner et al., 2002). The Young’s modulus E of the CNT is obtained from Eq. (3.8) as pﬃﬃﬃ 2= 3 Et ¼ , (3.11) 1 þ 8B 2 2 ðq V =qr ij Þ0 where the Young’s modulus appears together with the CNT thickness t since the strain energy density W in Eq. (3.4) is the strain energy per unit area. For small deformation, Eq. (3.7) gives the following approximate but analytical relation between the change of CNT radius DR and the internal pressure p (e.g., Timoshenko and Goodier, 1969) 2 3 pﬃﬃﬃ pR2 1 85 3 24 . (3.12) pR ¼ DR þ 2 2 Et ðq V=qr 2 Þ0 B ij The above equation is approximate but analytical, contrary to the numerical but accurate solution in Eq. (3.7). Similarly, both the numerical (but accurate) and analytical (but approximate) solutions are also obtained for continuum models in the following. ARTICLE IN PRESS Y.L. Chen et al. / J. Mech. Phys. Solids 56 (2008) 3224–3241 3229 3.2.2. Continuum modeling of hydrogen molecules The average spacing between hydrogen molecules, which is an important parameter in hydrogen storage, is obtained analytically in terms of the pressure p in this section. The Virial stress widely used in molecular dynamics simulations gives the stress tensor at the location ri of particle i as (McLellan, 1974; Tsai, 1979; Rowlinson and Widom, 1982) 0 1 [email protected] 1X (3.13) s¼ mi u_ i u_ i þ r f A, 2 jðaiÞ ij ij O where O is average volume per particle, mi and u_ i are the mass and velocity of particle i, respectively, rij ¼ rjri is the interatomic relative position vector in the current conﬁguration, fij is the interparticle force applied on particle i by particle j, and the summation is for all particles interacting with particle i. For the pair potential such as Lennard–Jones potential in Eq. (2.2) that depends only on the length r ij ¼ rij , f ij ¼ qV LJ dV LJ rij ¼ , qrij dr ij r ij (3.14) which is parallel to rij. For the system at relatively low temperature, the kinetic energy can be omitted, and the Virial stress in Eq. (3.13) then becomes s¼ 1 X 1 dV LJ r r . 2O jðaiÞ r ij dr ij ij ij (3.15) The internal pressure is p¼ 1 X dV LJ r . 6O jðaiÞ ij dr ij (3.16) For the limit of most closely packed hydrogen (AB stacking) illustrated in Fig. 4, there are 12 molecules surrounding each molecule, and their spacing is denoted by dH2 H2 . The volume per hydrogen molecule is pﬃﬃﬃ 2 3 d O¼ . (3.17) 2 H2 2H2 For the Lennard–Jones potential, Eq. (3.16) gives the following analytical relation to determine the spacing between hydrogen molecules dH2 H2 in terms of the internal pressure p: " pﬃﬃﬃ # 48 2H2 2H2 sH2 2H2 15 sH2 2H2 9 2 p¼ . (3.18) dH2 H2 dH2 2H2 s3H2 2H2 pﬃﬃﬃ The spacing dH2 H2 is 6 2sH2 H2 at the vanishing pressure p ¼ 0, and decreases as the pressure p increases, as shown in Fig. 5 for the (5,5) CNT. The atomistic model, also shown in Fig. 5, agrees very well with Eq. (3.18), and therefore validates this relation established from the Virial stress. Eq. (3.18) cannot be solved analytically to give the spacing dH2 H2 in terms of the pressure. An approximate but analytical expression can be obtained by neglecting ðsH2 2H2 =dH2 2H2 Þ9 in Eq. (3.18) since the repulsive term ðsH2 2H2 =dH2 2H2 Þ15 dominates as the internal pressure increases. The spacing dH2 H2 can then be approximated by dH2 2H2 !1=15 pﬃﬃﬃ 96 2H2 2H2 s12 H2 2H2 p . Fig. 4. Schematic diagrams of closely packed hydrogen molecules. (3.19) ARTICLE IN PRESS 3230 Y.L. Chen et al. / J. Mech. Phys. Solids 56 (2008) 3224–3241 80 70 Atomistic model (AFEM) Pressure (GPa) 60 50 Analytical relation (3.14) between H2 spacing and pressure 40 30 20 10 0 0.23 0.24 0.25 0.26 dH2-H2 (nm) 0.27 0.28 Fig. 5. The pressure inside the single-wall (5,5) carbon nanotube versus the equilibrium spacing between hydrogen molecules inside the nanotube. The results are shown for both the continuum model [Eq. (3.18)] and atomistic model (AFEM). 3.2.3. Continuum model of interactions between the CNT and hydrogen molecules The average spacing dC2H2 between the CNT wall and nearest hydrogen molecules, which is another important parameter in hydrogen storage, is obtained analytically in terms of the pressure p in this section. Jiang et al. (2006) established a cohesive law between a CNT and polymer molecules due to van der Waals interactions. By replacing polymer molecules with H2, it is also applicable to interactions between a CNT and hydrogen molecules " # sC2H2 4 2 sC2H2 10 , (3.20) p ¼ 2pO1 rC C2H2 s2C2H2 5 dC2H2 dC2H2 where rC is the number of carbon pﬃﬃﬃ atoms per2unit area of the CNT, and is related to the equilibrium bond length of carbon r0 ¼ 0.142 nm by rC ¼ 4=ð3 3r 20 Þ R=ðR þ DRÞ . The above equation then becomes " # pﬃﬃﬃ 2 C2H2 s2C2H2 2 sC2H2 10 sC2H2 4 8 2p R , (3.21) p ¼ pﬃﬃﬃ 3 5 dC2H2 dC2H2 3 3 R þ DR r2 d 0 H2 2H2 from Eqs. (3.7) and where the change of CNT radius DR and the spacing between hydrogen molecules dH2 2H2 are obtained pﬃﬃﬃﬃﬃﬃﬃﬃﬃ (3.18), respectively, or from Eqs. (3.12) and (3.19) for small deformation. The spacing dC2H2 is 6 2=5sC2H2 at the vanishing pressure p ¼ 0, and decreases as the pressure p increases, as shown in Fig. 6 for the (5,5) CNT. The atomistic model, also shown in Fig. 6, agrees well with Eq. (3.21) and therefore provides validation. Eq. (3.21) cannot be solved analytically to give the spacing dC2H2 in terms of the pressure. An approximate but analytical expression can be obtained by neglecting ðsC2H2 =dC2H2 Þ4 in Eq. (3.21) since the repulsive term ðsC2H2 =dC2H2 Þ10 dominates as the internal pressure increases. The spacing dC2H2 can then be approximated by " pﬃﬃﬃ #1=10 2 C2H2 s12 16 2p R C2H2 1 pﬃﬃﬃ . (3.22) dC2H2 3 p 15 3 R þ DR r2 d 0 H2 H2 3.2.4. Concentration of hydrogen molecules in a single-wall CNT For the CNT of radius R+DR, the hydrogen molecules can only be stored within the volume of radius R þ DR dC2H2 . The number of hydrogen molecules per unit length of the CNT is pðR þ DR dC2H2 Þ2 O1 . The number of hydrogen molecules per unit volume of the single-wall CNT is then 2 pﬃﬃﬃ pðR þ DR dC2H2 Þ2 O1 R þ DR dC2H2 2 NH ¼ ¼ , (3.23) 3 R þ DR pðR þ DRÞ2 d H2 2H2 where DR, dH2 2H2 and dC2H2 are obtained numerically from Eqs. (3.7), (3.18) and (3.21), respectively. As shown in Fig. 7 for the (5,5) CNT, NH increases as the internal pressure p increases. The curve stops at the peak pressure pmax ¼ 73.7 GPa obtained from Fig. 2. This gives the maximum hydrogen storage 31.3 nm3 in the (5,5) CNT. As shown in Fig. 7, the continuum model agrees reasonably well with the atomistic model, but the latter gives a smaller maximum hydrogen storage 25.6 nm3 denoted by the rightmost data point. ARTICLE IN PRESS Y.L. Chen et al. / J. Mech. Phys. Solids 56 (2008) 3224–3241 3231 80 70 Pressure (GPa) 60 Atomistic model (AFEM) 50 Analytical relation (3.17) between C-H2 spacing and pressure 40 30 20 10 0 0.18 0.19 0.20 0.21 0.22 0.23 dC-H2 (nm) 0.24 0.25 Fig. 6. The pressure inside the single-wall (5,5) carbon nanotube versus the equilibrium spacing between a hydrogen molecule and the nanotube. The results are shown for both the continuum model [Eq. (3.21)] and atomistic model (AFEM). Atomistic model (AFEM) Continuum model Analytical relation 30 31.3nm-3 (5,5) CNT NH (nm-3) 25 24.2nm-3 20 13.9nm-3 15 Bundle of (5,5) CNT Eq. (3.22) 10 10.1nm-3 5 Eq. (4.2) pmax = 73.7GPa 0 0 10 20 30 40 50 Pressure (GPa) 60 70 80 Fig. 7. The number of hydrogen molecules per unit volume versus the pressure inside the single-wall (5,5) carbon nanotubes or their bundles. The results are shown for the continuum model, atomistic model (AFEM) and (approximate) analytical solution [Eq. (3.26) for single-wall carbon nanotubes and Eq. (4.2) for their bundles]. The peak pressure is obtained from Fig. 2 as 73.7 GPa. For (n,n) armchair CNTs, the CNT radius R is given by R ¼ 0:0678n ðnmÞ. (3.24) Similar to Fig. 2, the peak pressure pmax for (n,n) armchair CNTs is also obtained and shown versus the CNT radius R in Fig. 8. It is inversely proportional to R, and is well approximated by pmax ¼ 25:6 GPa nm. R (3.25) The maximum hydrogen storage for the above peak pressure is shown versus the CNT radius R in Fig. 9. It initially increases with R, reaches the peak 65.7 nm3 at the (31,31) CNT (R ¼ 2.1 nm), and then decreases gradually. This maximum hydrogen storage (65.7 nm3) is more than twice of that for the (5,5) CNT, and exceeds the goals of hydrogen storage, as to be discussed in Section 6. However, single-wall CNTs larger than (30,30) may self collapse due to van der Waals interactions (Liu et al., 2004b). Therefore, for hydrogen storage in single-wall CNTs, it is optimal to use the largest one [i.e., (30,30)] without self collapse. ARTICLE IN PRESS 3232 Y.L. Chen et al. / J. Mech. Phys. Solids 56 (2008) 3224–3241 70 Peak pressure (GPa) 60 50 Triple-wall CNTs 40 Double-wall CNTs 30 20 10 Single-wall CNTs 0 0 1 2 3 4 R (nm) 5 6 7 Fig. 8. The peak pressure versus the radius of (inner or innermost) carbon nanotube. 70 Single-wall CNTs 60 Eq. (3.27) Bundle of single-wall CNTs NH (nm-3) 50 40 30 Eq. (4.3) Continuum model Analytical relation 20 10 0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0 4.5 5.0 5.5 6.0 R (nm) Fig. 9. The maximum hydrogen storage (at the peak pressure) versus the radius of single-wall nanotubes or their bundles. The results are shown for the continuum model and (approximate) analytical solution [Eq. (3.27) for single-wall carbon nanotubes and Eq. (4.3) for their bundles]. 3.2.5. Analytical solution The substitution of approximate but analytical relations (3.12), (3.19) and (3.22) into Eq. (3.23) gives the following analytical expression for the number of hydrogen molecules per unit volume of the CNT: 2 32 !1=10 17=50 1=10 ðC2H2 s12 2 p C2H2 Þ 7 pﬃﬃﬃ !1=5 6 1=50 7 6 5r 20 3 ðH2 2H2 s12 p 6 7 H2 2H2 Þ NH ¼ 61 7 6 7 24H2 2H2 s12 pR 6=5 H2 2H2 4 5 2=25 p R 1þ Et " #2 0:270 ¼ 45:0p1=5 1 , p2=25 Rð1 þ 0:00267pRÞ6=5 (3.26) where Et is given in Eq. (3.11), and the units of p, R and NH are GPa, nm and nm3, respectively. The above analytical expression, also shown in Fig. 7 for the (5,5) CNT, agrees well with the continuum and atomistic models. [Here, as well as the rest of the paper, ‘‘continuum model’’ refers to the numerical but accurate solution, while ‘‘analytical relation’’ refers to the approximate solution.] The curve also stops at the peak pressure pmax ¼ 73.7 GPa obtained from Fig. 2, which gives the maximum hydrogen storage 24.2 nm3 in the (5,5) CNT. It is smaller than 31.3 nm3 given by the continuum model, but is very close to 25.6 nm3 given by the atomistic model. ARTICLE IN PRESS Y.L. Chen et al. / J. Mech. Phys. Solids 56 (2008) 3224–3241 3233 For other (n,n) armchair CNTs, the substitution of peak pressure in Eq. (3.25) into the above equation gives the maximum hydrogen storage 86:1 0:193 2 NH ¼ 1=5 1 23=25 , (3.27) R R where the units of R and NH are nm and nm3, respectively. The above equation gives a maximum hydrogen storage 60.5 nm3 at the CNT radius R ¼ 2.1 nm. As shown in Fig. 9, it is slightly lower than the results from the continuum model, but may have better agreement with the atomistic model. 4. Hydrogen storage in the bundle of single-wall CNTs The hydrogen storage in single-wall CNTs involves many tubes, which may form CNT bundles. Fig. 10 shows a schematic diagram of an idealized CNT bundle. For relatively large tubes, the equilibrium spacing between CNTs is approximately the same as the characteristic length sC2C for the van der Waals interactions (Huang et al., 2006; Lu et al., 2007). The number of hydrogen molecules per unit volume of the CNT bundle is then obtained by modifying the volume in Eq. (3.23) as 0 12 pﬃﬃﬃ pðR þ DR dC2H2 Þ2 O1 2 p BR þ DR dC2H2 C p ﬃﬃﬃ NH ¼ pﬃﬃﬃ ¼ . (4.1) @ A 3 sC2C 2 2 3 R þ DR þ sC2C d H 2H 2 2 2 3 R þ DR þ 2 2 It is shown versus the internal pressure p in Fig. 7 for the bundle of (5,5) CNTs. The curve stops at the peak pressure pmax ¼ 73.7 GPa. This gives the maximum hydrogen storage in the bundle of (5,5) CNTs as 13.9 nm3, which is much smaller than 31.3 nm3 for the (5,5) CNT, and does not reach the goals of hydrogen storage set by the US Department of Energy. As shown in Fig. 7, the continuum model above agrees well with the atomistic model, but overestimates the maximum hydrogen storage since the atomistic model gives 11.0 nm3 denoted by the rightmost data point. The curves for the CNT bundle are lower than those for single-wall CNTs in Fig. 7 because of the spacing between CNTs in the bundle, which increases the volume for the same number of hydrogen molecules inside CNTs. Fig. 9 shows the maximum hydrogen storage versus the radius R of the (n,n) armchair CNTs in the bundle. The curve reaches the peak 53.9 nm3 for the bundle of (55,55) CNTs (R ¼ 3.73 nm), which exceeds the goals of hydrogen storage, as to be discussed in Section 6. Since single-wall CNTs larger than the (30,30) CNT may self collapse (Liu et al., 2004b), it is optimal to use the bundle of largest CNTs [i.e., (30,30), R ¼ 2.1 nm] without self collapse. The corresponding maximum hydrogen storage is only slightly smaller, 51.9 nm3. The substitution of approximate but analytical relations (3.12), (3.19) and (3.22) into Eq. (4.1) gives the following analytical expression for the number of hydrogen molecules per unit volume of the bundle of CNTs: 1=5 8 17=50 1=10 ðC2H s12 Þ1=10 92 2 C2H2 p > > p p ﬃﬃ p2ﬃﬃ p > > 12 < 5r 20 3 ðH2 2H2 s12 Þ1=50 = 2 3 24H2 2H2 sH 2H pR H2 2H2 2 2 NH ¼ 1þ 2 1=5 > > Et sCC > > ; : 1 þ pR p2=25 R 1 þ pR Et þ 2R Et ¼ " 40:8p1=5 2 ðR þ 0:00267pR2 þ 0:171Þ2 R þ 0:00267pR 0:270 p2=25 ð1 þ 0:00267pRÞ1=5 #2 , Fig. 10. Schematic diagram of the bundle of single-wall carbon nanotubes. (4.2) ARTICLE IN PRESS 3234 Y.L. Chen et al. / J. Mech. Phys. Solids 56 (2008) 3224–3241 where Et is given in Eq. (3.11), and the units of p, R and NH are GPa, nm and nm3, respectively. The above analytical expression, also shown in Fig. 7 for the bundle of (5,5) CNTs, agrees well with the continuum and atomistic models. The curve also stops at the peak pressure pmax ¼ 73.7 GPa (from Fig. 2) to give the maximum hydrogen storage 10.1 nm3 in the bundle of (5,5) CNTs, which is smaller than 13.9 nm3 from the continuum model but is close to 11.0 nm3 given by the atomistic model. For the bundle of (n,n) armchair CNTs, the substitution of peak pressure in Eq. (3.25) into the above equation gives the maximum hydrogen storage !2 78:1 0:206R2=25 þ 0:171 NH ¼ 1=5 1 , (4.3) 1:07R þ 0:171 R where the units of R and NH are nm and nm3, respectively. Eq. (4.3) gives a maximum hydrogen storage 49.0 nm3 for the bundle of CNTs with radii R ¼ 3.6 nm. As shown in Fig. 9, it is slightly lower than the results from the continuum model, but has better agreement with the atomistic model. For the maximum CNT (30,30) (R ¼ 2.1 nm) without self collapse, Eq. (4.3) gives 47.4 nm3, which is close to 51.9 nm3 given by the continuum model. 5. Hydrogen storage in multi-wall CNTs 5.1. Double-wall CNTs Fig. 11(a) shows the atomistic model for hydrogen storage in double-wall CNTs of radii R1 and R2. The covalent bonds between carbon atoms on the same CNT wall are characterized by the interatomic potential in Eq. (2.1). The carbon atoms from different CNT walls have the van der Waals interactions in Eq. (2.2), and so do carbon atoms and hydrogen molecules inside the CNT. Fig. 11(b) shows the continuum model to represent the inner and outer CNTs by thin shells of radii R1 and R2. The hydrogen molecules are still represented by the internal pressure p (on the inner shell). The van der Waals interaction between shells is characterized by the cohesive law for multi-wall CNTs (Lu et al., 2007), which gives the force–separation relation between two CNT walls from the van der Waals interactions. The equilibrium spacing between CNT walls is the van der Waals parameter sC2C, i.e., R2 ¼ R1 þ sC2C . Let R1 þ DR1 and R2 þ DR2 denote the radii of inner and outer walls after the internal pressure p is imposed. The energy (per unit length of the CNT) stored between two CNT walls due to van der Waals interactions is (Lu et al., 2007) " 10 4 # 2 sC2C sC2C , (5.1) 2p2 ðR2 þ DR2 þ R1 þ DR1 ÞrC1 rC2 C2C s2C2C 5 R2 þ DR2 R1 DR1 R2 þ DR2 R1 DR1 where rC 1 and rC 2 are the numbers of carbon atoms per unit area of the inner and outer CNTs, respectively, and are related to the equilibrium bond length of carbon r 0 ¼ 0:142 nm by 2 4 Ri rCi ¼ pﬃﬃﬃ 2 ði ¼ 1; 2Þ: 3 3r 0 Ri þ DRi The energy stored in each CNT wall is obtained in the same way as described in Eqs. (3.1)–(3.6). The total energy is the sum of energy in each CNT and the energy between CNT walls in Eq. (5.1) due to van der Waals interactions. The minimization of total energy gives the change of inner and outer CNT radii DR1 and DR2 in terms of the internal pressure p. Fig. 12 shows the internal pressure p in the CNT versus the percentage of change of CNT radii, DR1 =R1 and DR2 =R2 , obtained from both atomistic and continuum models for the (5,5)(10,10) double-wall CNT. The curve for the inner (5,5) CNT is higher than that for the (5,5) single-wall CNT in Fig. 2 due to van der Waals interactions between two CNT walls. The peak pressure for the (5,5)(10,10) double-wall CNT is 89.3 GPa (at which the inner CNT starts to display softening behavior), which is signiﬁcantly larger than pmax ¼ 73.7 GPa for the (5,5) single-wall CNT (Fig. 2). The continuum model agrees well with the atomistic model. Only the peak pressure given by the continuum model is slightly higher than the atomistic model. The analyses in Sections 3.2.2 and 3.2.3 still hold. The spacing between hydrogen molecules dH2 2H2 is determined from Eq. (3.18) [or Eq. (3.19)]. The spacing between the inner CNT wall and nearest hydrogen molecules dC2H2 is obtained from Eq. (3.21) [or Eq. (3.22)] with R and DR replaced by R1 and DR1, respectively. For the inner CNT of radius R1 þ DR1 , the hydrogen molecules can only be stored within the volume of radius R1 þ DR1 dC2H2 . The number of hydrogen molecules per unit length of the CNT is pðR1 þ DR1 dC2H2 Þ2 O1 . The number of hydrogen molecules per unit volume of the double-wall CNT is then 2 pﬃﬃﬃ pðR1 þ DR1 dC2H2 Þ2 O1 R1 þ DR1 dC2H2 2 NH ¼ ¼ , (5.2) 2 3 R þ D R 2 2 pðR2 þ DR2 Þ d H2 H2 where DR1 and DR2 are determined from the minimization of total energy, and dH2 2H2 and dC2H2 are obtained numerically from Eqs. (3.18) and (3.21), respectively. As shown in Fig. 13 for the (5,5)(10,10) double-wall CNT, NH increases ARTICLE IN PRESS Y.L. Chen et al. / J. Mech. Phys. Solids 56 (2008) 3224–3241 3235 Hydrogen Carbon Fig. 11. Schematic diagrams of hydrogen storage in double-wall carbon nanotubes: (a) atomistic model (AFEM), in which carbon atoms and hydrogen molecules are discrete; and (b) continuum model, in which carbon nanotubes are represented by a continuum shell, while hydrogen molecules are represented by the internal pressure. (5,5)(10,10) double-wall CNT 100 Peak pressure 90 Pressure (GPa) 80 70 Outer CNT Inner CNT 60 50 40 30 20 Atomistic model (AFEM) Continuum model 10 0 0.00 0.02 0.04 0.06 0.08 0.10 0.12 0.14 0.16 ΔR/R Fig. 12. The pressure inside the (5,5)(10,10) double-wall carbon nanotube versus the percentage change of inner and outer nanotube radii for the atomistic (AFEM) and continuum models. The peak pressure is denoted. as the internal pressure p increases. The curve stops at the peak pressure 89.3 GPa. This gives the maximum hydrogen storage in the (5,5)(10,10) double-wall CNT as 11.0 nm3, which is signiﬁcantly smaller than 31.3 nm3 for (5,5) single-wall CNT and also smaller than 13.9 nm3 for the bundle of (5,5) single-wall CNTs (Fig. 7), and does not ARTICLE IN PRESS 3236 Y.L. Chen et al. / J. Mech. Phys. Solids 56 (2008) 3224–3241 12 11.0nm-3 Atomistic model (AFEM) Continuum model 10 (5,5)(10,10) double-wall CNT NH (nm-3) 8 6 5.1nm-3 (5,5)(10,10)(15,15) triple-wall CNT 4 2 pmax = 90.8GPa pmax = 89.3GPa 0 0 10 20 30 50 40 60 Pressure (GPa) 70 80 90 Fig. 13. The number of hydrogen molecules per unit volume versus the pressure inside the (5,5)(10,10) double-wall and (5,5)(10,10)(15,15) triple-wall carbon nanotubes. The results are shown for the continuum model and atomistic model (AFEM). The peak pressures for double- and triple-wall carbon nanotubes are denoted. reach the goals of hydrogen storage. Fig. 13 also shows the results from the atomistic model, which agree well with the continuum model but give a smaller maximum hydrogen storage 9.0 nm3 denoted by the rightmost data point. For (n,n)(n+5,n+5) double-wall CNTs, the radii R1 and R2 of inner and outer CNTs are still given by Eq. (3.24), and their spacing is approximately sC2C. The peak pressure pmax for double-wall CNTs is shown versus the radius R1 of the inner CNT in Fig. 8. It is approximately proportional to the inverse of average radius R̄ ¼ ðR1 þ R2 Þ=2, pmax ¼ 48:8 GPa nm: R̄ (5.3) For the above pmax, Fig. 14 shows the maximum hydrogen storage versus the inner radius R1 of double-wall CNT. The curve reaches the peak 63.8 nm3 at the (70,70)(75,75) double-wall CNT (R1 ¼ 4.7 nm). This maximum hydrogen storage is almost six times 11.0 nm3 for the (5,5)(10,10) double-wall CNT, and exceeds the goals of hydrogen storage, as to be discussed in Section 6. However, double-wall CNTs larger than the (36,36)(41,41) CNT may self collapse due to the van der Waals interactions (Xiao et al., 2007). Therefore, for hydrogen storage in double-wall CNTs, it is optimal to use the largest one [i.e., (36,36)(41,41)] without self collapse. Similar to Section 3.2.1, the change of inner and outer CNT radii DR1 and DR2 can be obtained analytically for small deformation as ( ) ( ) 1 þ lðR1 þ R2 ÞR2 pR21 DR1 1 , (5.4) ¼ lðR1 þ R2 ÞR2 DR2 Et 1 þ lðR1 þ R2 Þ2 where l ¼ 128pC2C =ð9r 40 EtÞ and Et is given in Eq. (3.11). The substitution of the analytical but approximate relations (5.3), (5.4), (3.19) and (3.22) into Eq. (5.2) leads to the following analytical expression for the number of hydrogen molecules per unit volume of double-wall CNT: 2=25 NH ¼ 97:9 ðR1 w6=5 0:198R̄ Þ2 h i , 1=5 2 2 R22 R̄ w2=5 1 þ 0:0294R21 =ð1 þ 0:448R̄ Þ (5.5) 2 where R̄ ¼ ðR1 þ R2 Þ=2 is the average radius, w ¼ 1 þ 0:130ðR1 =R̄Þð1 þ 0:224R2 R̄Þ=ð1 þ 0:448R̄ Þ, and the units of R1, R2, R̄ and NH are nm, nm, nm and nm3, respectively. Eq. (5.5) gives a maximum hydrogen storage 58.2 nm3 for the inner CNT radius R1 ¼ 4.3 nm. As shown in Fig. 14, it is slightly smaller than that for the continuum model. 5.2. Multi-wall CNTs The equilibrium spacing between CNT walls is the van der Waals parameter sC2C, i.e., R2 ¼ R1 þ sC2C , R3 ¼ R2 þ sC2C , y Let R1 þ DR1 , R2 þ DR2 , R3 þ DR3 , y denote the radii of CNT walls after the internal pressure p is imposed. The energy ARTICLE IN PRESS Y.L. Chen et al. / J. Mech. Phys. Solids 56 (2008) 3224–3241 70 3237 Double-wall CNTs 65 60 55 50 NH (nm-3) 45 Triple-wall CNTs 40 35 30 Continuum model 25 Analytical relation (5.5) 20 15 10 5 0 0 1 2 3 4 5 R1 (nm) 6 7 8 9 Fig. 14. The maximum hydrogen storage (at the peak pressure) versus the (inner or innermost) radius of double- and triple-wall carbon nanotubes. The results are shown for the continuum model and (approximate) analytical solution [Eq. (5.5)]. (per unit length of the CNT) stored between CNTs walls due to van der Waals interactions is 9 8 ðRiþ1 þ DRiþ1 þ Ri þ DRi ÞrCi rCiþ1 > > > > < " # X 10 4 = 2 2 s s , 2p CC sCC C2C C2C 2 > > 5 > i > ; : Riþ1 þ DRiþ1 Ri DRi Riþ1 þ DRiþ1 Ri DRi (5.6) pﬃﬃﬃ 2 where rCi ¼ 4= 3 3r 20 Ri =ðRi þ DRi Þ . The energy stored in each CNT wall is obtained in the same way as described in Eqs. (3.1)–(3.6). The total energy is the sum of energy in each CNT and the energy between CNT walls given in Eq. (5.6) due to van der Waals interactions. The minimization of total energy gives the change of CNT radii DRi (i ¼ 1, 2, 3, y) in terms of the internal pressure p. The analyses in Sections 3.2.2 and 3.2.3 still hold. The number of hydrogen molecules per unit volume of the CNT is NH ¼ pðR1 þ DR1 dC2H2 Þ2 O1 R1 þ DR1 dC2H2 ¼ 2 Rm þ DRm pðRm þ DRm Þ 2 pﬃﬃﬃ 2 3 dH2 2H2 , (5.7) where Rm is the radius of outermost CNT. It is shown in Fig. 13 versus the internal pressure p for the (5,5)(10,10)(15,15) triple-wall CNT. The peak pressure 90.8 GPa is very close to 89.3 GPa for the (5,5)(10,10) double-wall CNT, which means that the CNTs beyond the innermost two have essentially no effect. The maximum hydrogen storage in the (5,5)(10,10)(15,15) triple-wall CNT is only 5.1 nm3. For (n,n)(n+5,n+5)(n+10,n+10) triple-wall CNTs, the peak pressure pmax is shown versus the radius R1 of the innermost CNT in Fig. 8. It is approximately proportional to the inverse of average radius R̄ ¼ ðR1 þ R2 þ R3 Þ=3 pmax ¼ 77:3 GPa nm. R̄ (5.8) Fig. 14 shows the maximum hydrogen storage versus R1. The curve reaches the peak 63.2 nm3 at the (110,110)(115,115)(120,120) triple-wall CNT (R1 ¼ 7.5 nm). This exceeds the goals of hydrogen storage, as to be discussed in Section 6. However, triple-wall CNTs larger than the (42,42)(47,47)(52,52) CNT may self collapse due to the van der Waals interactions (Xiao et al., 2007). Therefore, for hydrogen storage in triple-wall CNTs, it is optimal to use the largest one [i.e., (42,42)(47,47)(52,52)] without self collapse. The curve for triple-wall CNTs is lower than its counterpart for double-wall CNTs at the small radius R1 in Fig. 14, but this trend is reversed at relatively large radius. This is due to two competing effects as the number of walls increases. One is the volume increase (for the same number of hydrogen molecules), which reduces the maximum hydrogen storage. The other is that the peak pressure in the inner(most) wall increases with the increase of number of walls, which allows more hydrogen molecules inside the inner(most) wall. These two effects dominate at small and large radii, respectively, which is ARTICLE IN PRESS 3238 Y.L. Chen et al. / J. Mech. Phys. Solids 56 (2008) 3224–3241 why the curves in Fig. 14 cross. In fact, the comparison of the curve for single-wall CNT in Fig. 9 with the curves for doubleand triple-wall CNTs shows the same trend. 6. Discussion and concluding remarks The maximum hydrogen storage shown in Figs. 9 and 14 corresponds to the limit state at which the (inner or innermost) CNT starts to fracture (or exhibit softening behavior). The strain (in the circumferential direction) is about 16.6%. The cyclic storage and release of hydrogen in CNTs requires the strain be signiﬁcantly less than this level. One goal of hydrogen storage set by the US Department of Energy is 62 kg H2/m3 of hydrogen (Dillon et al., 1997), which can be converted to NH ¼ 18:7 nm3 using the atomic weights. This requires the internal pressure p ¼ 35.5 GPa from Fig. 7 for the (5,5) CNT, which corresponds to the strain in the circumferential direction ¼ DR=R ¼ 4:4%. For the bundle of (5,5) CNTs shown in Fig. 7 as well as (5,5)(10,10) double-wall and (5,5)(10,10)(15,15) triple-wall CNTs shown in Fig. 13, the required hydrogen storage 18.7 nm3 can never be reached even when the (inner or innermost) CNT fractures. Fig. 15 shows the strain (in the circumferential direction) in the CNT to achieve 62 kg H2/m3 of hydrogen versus n for (n,n) single-wall CNTs and their bundles, (n,n)(n+5,n+5) double-wall and (n,n)(n+5,n+5)(n+10,n+10) triple-wall CNTs. As the CNT radius increases, the strain in the CNT to achieve 62 kg H2/m3 decreases. The strain is zero for single-wall CNTs larger than (14,14), which means single-wall CNTs between (14,14) and (30,30) can achieve 62 kg H2/m3 without the strain and do not self collapse. For the bundle of CNTs, the strain is zero for CNTs larger than (22,22) such that any bundle of CNTs between (22,22) and (30,30) can achieve 62 kg H2/m3 without the strain and do not self collapse. For double-wall CNTs, this range becomes (25,25) to (36,36) (for the inner CNT), while for triple-wall CNTs this range is (37,37) to (42,42) (for the innermost CNT). For the other goal 6.5wt% of hydrogen storage set by the US Department of Energy (Dillon et al., 1997), the corresponding NH can be similarly obtained using the atomic weights and CNT radius. Fig. 16 shows the strain (in the circumferential direction) to achieve 6.5 wt% H2 versus n for (n,n) single-wall CNTs, which is also the same as the bundle of CNTs, and for (n,n)(n+5,n+5) double-wall and (n,n)(n+5,n+5)(n+10,n+10) triple-wall CNTs. As the CNT radius increases, the strain in the CNT to achieve 6.5 wt% H2 decreases. It is zero for single-wall CNTs (and their bundles) larger than (19,19) such that single-wall CNTs between (19,19) and (30,30) can achieve 6.5 wt% H2 without the strain and do not self collapse. For double-wall CNTs, this range becomes (32,32) to (36,36) (for the inner CNT), while for triple-wall CNTs this range does not exist anymore. In order to achieve both goals of 62 kg H2/m3 and 6.5 wt% H2 for hydrogen storage, CNTs display different behavior depending on their radii, as shown in Table 1. (1) (2) (3) (4) tiny CNTs fracture to reach the goals of hydrogen storage (2nd column); small CNTs experience strains upon hydrogen storage (3rd column); medium CNTs have no strain and do not self collapse (4th column); and large CNTs may self collapse upon the release of hydrogen (5th column). The corresponding ranges of radii are also shown in Table 1. For the ‘‘small’’ CNTs in the 3rd column of Table 1, even though the strains are below the fracture strain of CNTs (16.6%), defects may nucleate in the form of Stone–Wales transformation (901rotation of a C–C bond) at a much smaller 0.16 0.14 0.12 Bundle of single-wall CNTs 0.10 Strain 62 kg H2 /m3 Single-wall CNTs 0.08 Double-wall CNTs 0.06 0.04 Triple-wall CNTs 0.02 0.00 0 5 10 15 20 n 25 30 35 Fig. 15. The strain in the (inner or innermost) carbon nanotube to reach 62 kg H2/m3, the goal for hydrogen storage set by the US Department of Energy. The strain is shown versus n for single-, double- and triple-wall carbon nanotubes and their bundles, where (n,n) represent the charality of armchair carbon nanotubes. ARTICLE IN PRESS Y.L. Chen et al. / J. Mech. Phys. Solids 56 (2008) 3224–3241 0.16 3239 6.5 wt% 0.14 Single-wall CNTs & Bundle of single-wall CNTs 0.12 Strain 0.10 0.08 Double-wall CNTs 0.06 0.04 Triple-wall CNTs 0.02 0.00 0 5 10 15 20 25 n 35 30 40 45 Fig. 16. The strain in the (inner or innermost) carbon nanotube to reach 6.5wt%, the other goal for hydrogen storage set by the US Department of Energy. The strain is shown versus n for single-, double- and triple-wall carbon nanotubes and their bundles, where (n,n) represent the charality of armchair carbon nanotubes. Table 1 Behavior of different carbon nanotubes to achieve the goals of hydrogen storage (62 kg H2/m3 and 6.5 wt%) Ranges of CNT charality and radius Fracture Strained No strain or self collapse Self collapse Single-wall CNTs (7,7) and down o0.47 nm (8,8) to (18,18) 0.54–1.2 nm (19,19) to (30,30) 1.3–2.0 nm (31,31) and up 42.1 nm Bundle of single-wall CNTs (7,7) and down o0.47 nm (8,8) to (21,21) 0.54–1.4 nm (22,22) to (30,30) 1.5–2.0 nm (31,31) and up 42.1 nm Double-wall CNTs (inner tube) (11,11) and down o0.75 nm (12,12) to (31,31) 0.81–2.1 nm (32,32) to (36,36) 2.2–2.4 nm (37,37) and up 42.5 nm Triple-wall CNTs (innermost tube) (16,16) and down o1.1 nm (17,17) to (41,41) 1.2–2.8 nm – – (42,42) and up 42.8 nm strain, around 5% (Nardelli et al., 1998a, b; Jiang et al., 2004; Song et al., 2006). Therefore, in order to avoid defect nucleation and self collapse, the suitable ranges for hydrogen storage are (10,10) to (30,30) for single-wall CNTs and their bundles, (17,17) to (36,36) for (the inner tube of) double-wall CNTs, and (24,24) to (41,41) for (the innermost tube of) triple-wall CNTs. The hydrogen storage in zig–zag and chiral CNTs is also studied. The peak pressure is essentially independent of the charality, and is given by Eqs. (3.25), (5.3) and (5.8) for single-, double- and triple-wall (zig–zag and chiral) CNTs, respectively. For CNTs of the same radius, the maximum hydrogen storage in zig–zag CNTs is a few percent (o5%) higher than that in armchair CNTs, while the results for chiral CNTs are between those for armchair and zig–zag CNTs. The effect of ‘‘caps’’ at the two ends of the CNT is negligible. The peak pressure for CNTs with closed caps is slightly smaller (less than 1.5%) than that without caps, while the maximum hydrogen storage is less than 0.3% smaller. Hydrogen adsorption on the exterior surface of CNT is studied by modifying the model shown in Fig. 1 to introduce one layer of hydrogen molecules outside the CNT. The distances between this layer and the CNT and of hydrogen pﬃﬃﬃﬃﬃﬃﬃﬃﬃ between molecules are obtained from Eqs. (3.21) and (3.18) as dC2H2 p¼0 ¼ 6 2=5sC2H2 ¼ 0:274 nm and ﬃﬃﬃ p hydrogen dH2 2H2 p¼0 ¼ 6 2sH2 2H2 ¼ 0:332 nm, respectively. Fig. 17 shows the maximum hydrogen storage NH (at the peak internal pressure), with and without surface absorption, versus the CNT radius R for single-wall CNTs. The maximum hydrogen storage with surface absorption is in fact smaller than that without surface absorption because the former occupies a larger volume (corresponding to the radius R þ DR þ dC2H2 , as opposed to R þ DR for the latter). This volume increase overwhelms the increase in the number of hydrogen molecules due to surface adsorption, and therefore leads to smaller maximum hydrogen storage. ARTICLE IN PRESS 3240 Y.L. Chen et al. / J. Mech. Phys. Solids 56 (2008) 3224–3241 70 Without surface absorption 65 60 NH (nm-3) 55 With surface absorption 50 45 40 35 Single-wall CNTs 30 25 20 0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0 4.5 5.0 5.5 6.0 R (nm) Fig. 17. The maximum hydrogen storage (at the peak pressure) versus the radius of single-wall nanotubes, with and without hydrogen absorption to the exterior surface of nanotubes. Heterogeneous carbon nanostructures, such as nanotube-derived carbon foam (Ding et al., 2007), CNTs doped by metals (Krasnov et al., 2007), and carbon nano-framework (Weck et al., 2007), have also been studied for hydrogen storage, and so has fullerene (Pupysheva et al., 2008). These heterogeneous carbon nanostructures and fullerene have shown improved hydrogen storage, but are beyond the scope of the present study. In summary, the following conclusions on hydrogen storage in CNTs are established in this paper. (1) The continuum models for hydrogen storage in CNTs have been established to account for the deformation of CNTs, the van der Waals interactions between hydrogen molecules and between hydrogen and CNTs. The continuum models agree well with the atomistic simulations without parameter ﬁtting. (2) For single-, double- and triple-wall CNTs and bundles of single-wall CNTs, the continuum models give analytical expressions of hydrogen storage (number of hydrogen molecules per unit volume) in terms of the CNT radius and pressure. The maximum hydrogen storage corresponding to the peak pressure far exceeds the goals of hydrogen storage (62 kg H2/m3 and 6.5wt% H2) set by the US Department of Energy. (3) Each type of CNTs (single-, double- and triple-wall, and bundle) can be categorized as tiny, small, medium and large CNTs as shown in Table 1. Tiny CNTs cannot achieve the above goals of hydrogen storage without fracture; small CNTs are strained during hydrogen storage; medium CNTs can achieve the above goals without the strain and do not self collapse; and large CNTs may self collapse upon the release of hydrogen. Acknowledgments B.L. acknowledges the support from National Natural Science Foundation of China (Grant nos. 10542001, 10702034 and 10732050). K.C.H. acknowledges the support from National Basic Research Program of China (973 Program) Grant no. 2007CB936803. Y.H. acknowledges the support from the NSF through Nano-CEMMS (Grant no. DMI03-28162) at the University of Illinois and ONR Composites for Marine Structures Program (Grant no. N00014-01-1-0205, Program Manager Dr. Y.D.S. Rajapakse). The supports from the NSFC and Ministry of Education of China are also acknowledged. References Allen, M.P., Tildesley, D.J., 1987. Computer Simulation of Liquids. Clarendon Press, Oxford. Born, M., Huang, K., 1954. Dynamical Theory of the Crystal Lattices. Oxford University Press, Oxford. Brenner, D.W., Shenderova, O.A., Harrison, J.A., Stuart, S.J., Ni, B., Sinnott, S.B., 2002. A second-generation reactive empirical bond order (REBO) potential energy expression for hydrocarbons. J. Phys.: Condens. Matter 14, 783–802. Chen, P., Wu, X., Lin, J., Tan, K.L., 1999. High H2 uptake by alkali-doped carbon nanotubes under ambient pressure and moderate temperatures. Science 285 (5424), 91–93. Cheng, H.-M., Yang, Q.-H., Liu, C., 2001. Hydrogen storage in carbon nanotubes. Carbon 39 (10), 1447–1454. Cheng, J., Yuan, X., Zhao, L., Huang, D., Zhao, M., Dai, L., Ding, R., 2004. GCMC simulation of hydrogen physisorption on carbon nanotubes and nanotube arrays. Carbon 42 (10), 2019–2024. Dai, G.P., Liu, C., Liu, M., Wang, M.Z., Cheng, H.M., 2002. Electrochemical hydrogen storage behavior of ropes of aligned single-walled carbon nanotubes. Nano Letters 2 (5), 503–506. Darkrim, F.L., Levesque, D., 1998. Monte Carlo simulations of hydrogen adsorption in single-walled carbon nanotubes. J. Chem. Phys. 109 (12), 4981–4984. Darkrim, F.L., Levesque, D., 2000. High adsorptive property of opened carbon nanotubes at 77 K. J. Phys. Chem. 104, 6773–6776. Darkrim, F.L., Malbrunot, P., Tartaglia, G.P., 2002. Review of hydrogen storage by adsorption in carbon nanotubes. Int. J. Hydrogen Energy 27 (2), 193–202. Dillon, A.C., Jones, K.M., Bekkedahl, T.A., Kiang, C.H., Bethune, D.S., Heben, M.J., 1997. Storage of hydrogen in single-walled carbon nanotubes. Nature 386, 377–379. ARTICLE IN PRESS Y.L. Chen et al. / J. Mech. Phys. Solids 56 (2008) 3224–3241 3241 Ding, F., Lin, Y., Krasnov, P.O., Yakobson, B.I., 2007. Nanotube-derived carbon foam for hydrogen sorption. J. Chem. Phys. 127 (16), 164703. Dodziuk, H., Dolgonos, G., 2002. Molecular modeling study of hydrogen storage in carbon nanotubes. Chem. Phys. Lett. 356 (1–2), 79–83. Frankland, S.J.V., Harik, V.M., Odegard, G.M., Brenner, D.W., Gates, T.S., 2003. The stress–strain behavior of polymer–nanotube composites from molecular dynamics simulation. Compos. Sci. Technol. 63, 1655–1661. Gao, H.J., Klein, P., 1998. Numerical simulation of crack growth in an isotropic solid with randomized internal cohesive bonds. J. Mech. Phys. Solids 46, 187–218. Gu, C., Gao, G.-H., Yu, Y.-X., Mao, Z.-Q., 2001. Simulation study of hydrogen storage in single walled carbon nanotubes. Int. J. Hydrogen Energy 26 (7), 691–696. Huang, Y., Wu, J., Hwang, K.C., 2006. Thickness of graphene and single-wall carbon nanotubes. Phys. Rev. B 74, (245413/1–9). Jiang, H., Feng, X.Q., Huang, Y., Hwang, K.C., Wu, P.D., 2004. Defect nucleation in carbon nanotubes under tension and torsion: Stone–Wales transformation. Comput. Methods Appl. Mech. Eng. 193 (30–32), 3419–3429. Jiang, L.Y., Huang, Y., Jiang, H., Ravichandran, G., Gao, H., Hwang, K.C., Liu, B., 2006. A cohesive law for carbon nanotube/polymer interfaces based on the van der Waals force. J. Mech. Phys. Solids 54, 2436–2452. Krasnov, P.O., Ding, F., Singh, A.K., Yakobson, B.I., 2007. Clustering of Sc on SWNT and reduction of hydrogen uptake: ab-initio all-electron calculations. J. Phys. Chem. C 111 (49), 17977–17980. Liu, B., Huang, Y., Jiang, H., Qu, S., Hwang, K.C., 2004a. The atomic-scale ﬁnite element method. Comput. Methods Appl. Mech. Eng. 193, 1849–1864. Liu, B., Yu, M.F., Huang, Y.G., 2004b. Role of lattice registry in the full collapse and twist formation of carbon nanotubes. Phys. Rev. B 70 (16), 161402. Liu, B., Jiang, H., Huang, Y., Qu, S., Yu, M.-F., 2005. Atomic-scale ﬁnite element method in multiscale computation with applications to carbon nanotubes. Phys. Rev. B 72 (3), (035435/1–8). Liu, C., Fan, Y.Y., Liu, M., Cong, H.T., Cheng, H.M., Dresselhaus, M.S., 1999. Hydrogen storage in single-walled carbon nanotubes at room temperature. Science 286 (5442), 1127–1129. Lu, W.B., Wu, J., Jiang, L.Y., Huang, Y., 2007. A cohesive law for multi-wall carbon nanotubes. Philos. Mag. 87, 2221–2232. McLellan, A.G., 1974. Virial theorem generalized. Am. J. Phys. 42, 239–243. Mu, S.-c., Tang, H.-l., Qian, S.-h., Pan, M., Yuan, R.-z., 2006. Hydrogen storage in carbon nanotubes modiﬁed by microwave plasma etching and Pd decoration. Carbon 44 (4), 762–767. Nardelli, M.B., Yakobson, B.I., Bernholc, J., 1998a. Brittle and ductile behavior in carbon nanotubes. Phys. Rev. Lett. 81, 4656–4659. Nardelli, M.B., Yakobson, B.I., Bernholc, J., 1998b. Mechanism of strain release in carbon nanotubes. Phys. Rev. B 57, R4277–R4280. Pupysheva, O.V., Farajian, A.A., Yakobson, B.I., 2008. Fullerene nanocage capacity for hydrogen storage. Nano Letters 8 (3), 767–774. Rajalakshmi, N., Dhathathreyan, K.S., Govindaraj, A., Satishkumar, B.C., 2000. Electrochemical investigation of single-walled carbon nanotubes for hydrogen storage. Electrochim. Acta 45, 4511–4515. Rowlinson, J.S., Widom, B., 1982. Molecular Theory of Capillarity. Clarendon Press, Oxford. Song, J., Jiang, H., Shi, D.L., Feng, X.Q., Huang, Y., Yu, M.F., Hwang, K.C., 2006. Stone–Wales transformation: precursor of fracture in carbon nanotubes. Int. J. Mech. Sci. 48 (12), 1464–1470. Timoshenko, S., Goodier, J.N., 1969. Theory of Elasticity, third ed. McGraw-Hill Book Co., Inc., New York. Tsai, D.H., 1979. The virial theorem and stress calculation in molecular dynamics. J. Chem. Phys. 70 (3), 1375–1382. Weck, P.F., Kim, E., Balakrishnan, N., Cheng, H.S., Yakobson, B.I., 2007. Designing carbon nanoframeworks tailored for hydrogen storage. Chem. Phys. Lett. 439, 354–359. Wu, J., Hwang, K.C., Huang, Y., 2008. An atomistic-based ﬁnite-deformation shell theory for single-wall carbon nanotubes. J. Mech. Phys. Solids 56, 279–292. Wu, X.B., Chen, P., Lin, J., Tan, K.L., 2000. Hydrogen uptake by carbon nanotubes. Int. J. Hydrogen Energy 25 (3), 261–265. Xiao, J., Liu, B., Huang, Y., Zuo, J., Hwang, K.C., Yu, M.F., 2007. Collapse and stability of single- and multi-wall carbon nanotubes. Nanotechnology 18, 395703. Yang, R.T., 2000. Hydrogen storage by alkali-doped carbon nanotubes—revisited. Carbon 38, 623–626. Ye, Y., Ahn, C.C., Witham, C., Fultz, B., Liu, J., Rinzler, A.G., Colbert, D., Smith, K.A., Smalley, R.E., 1999. Hydrogen adsorption and cohesive energy of single-walled carbon nanotubes. Appl. Phys. Lett. 74 (16), 2307–2309. Zhang, P., Huang, Y., Geubelle, P.H., Klein, P.A., Hwang, K.C., 2002. The elastic modulus of single-wall carbon nanotubes: a continuum analysis incorporating interatomic potentials. Int. J. Solid Struct. 39, 3893–3906. Zhang, P., Jiang, H., Huang, Y., Geubelle, P.H., Hwang, K.C., 2004. An atomistic-based continuum theory for carbon nanotubes: analysis of fracture nucleation. J. Mech. Phys. Solids 52, 977–998.